R ESEARCHARTICLEScienceAsia 47 (2021): 220–227doi: 10.2306/scienceasia1513-1874.2021.032Aluminum- and iron-engineered biochar fromsugarcane filter cake as phosphorus adsorbents andfertilizersNatcha Sornhirana , Jirapat Tuntrachanidaa , Prapapun Malacheya , Patchara Thongtuka ,Worachart Wisawapipata,b, , Surachet Aramraka , Nattaporn Prakongkepcabc Department of Soil Science, Faculty of Agriculture, Kasetsart University, Bangkok 10900 ThailandResearch Network of NANOTEC – KU on NanoCatalysts and NanoMaterials for Sustainable Energy andEnvironment, Kasetsart University, Bangkok 10900 ThailandOffice of Science for Land Development, Land Development Department, Bangkok 10900 ThailandCorresponding author, e-mail: [email protected] 30 Sep 2020Accepted 17 Feb 2021ABSTRACT: Reclamation of phosphorus (P) from wastewater using metal-engineered biochar and its reuses asphosphate fertilizers could be an eco-friendly and effective technology for the sustainability of environmental andagricultural systems. Herein, we studied the P removal capacity of filter cake-engineered biochar loaded with Al andFe and examined their available P release capability into the sand sample. The Al-biochar (63.7 mg/g) had a higher Pretention capacity than the Fe-biochar (33.2 mg/g). Over 45 days of the incubation, Al- and Fe-biochar incorporationsteadily or increasingly released adequate concentrations of available P to the sand sample. Furthermore, a considerableP fraction (99.4–99.8% of the total P) remained in all metal-biochar samples, suggesting that the metal biochar could bea long-term source of the available P pool. This study highlighted the potential use of Al- and Fe-biochar for providingavailable P availability in sandy soils.KEYWORDS: metal-engineered biochar, P sorption, sandy soilINTRODUCTIONBiochar is a carbon-rich material with high stabilityproduced by the carbonization of biomass underlimited oxygen [1, 2]. This material has variousbenefits such as promoting the water and nutrient retention capacity in soils and improving plantproductivity [1, 3]. Biochar is also documented asa low-cost and eco-friendly technology for reusingagricultural wastes to recover nutrients such asnitrate and phosphate from wastewaters that otherwise typically cause eutrophication in aquaticecosystems [4, 5]. Engineering biochar with metals has been an effective method, among severalapproaches, to elevate biochar chemical reactivityfor the removal of such pollutants from industrialwastewater [6–9]. The metal-engineered biocharafter wastewater P removal (P-laden biochar) isabundant in phosphate and has been proven forreuse and P-recycled fertilizer [7, 10].To date, different metals such as Al and Fehave been used to produce engineered biochar[7, 11, 12]. Precipitated metal (oxyhydr)oxides inwww.scienceasia.orgthe biochar framework could act as the main adsorbents for P. Al-biochar and Fe-biochar containingrespective metal oxides like gibbsite (AlOOH) andmagnetite (Fe2 O3 ) have also been documented asexcellent P adsorbents [11–13], but the informationon their effects on soil P availability is lacking.Soil phosphorus (P) availability is quite limitedin many soil types such as sandy soils [14, 15].Conversely, P limitation in sandy soil is inherentfrom its properties, in which commonly there arelow amounts of the clay-sized fraction with highchemical reactive sites for nutrient retention, whichcan promote nutrient losses through leaching bydrainage . Deficient available water holdingcapacity is also a severe constraint for sandy soils.Therefore, P-laden biochar could be a promisingmaterial that can resolve both P and water retentionissues for this soil type [17, 18].The filter cake is a by-product of the sugarcane industry with a high potential for engineeredbiochar production. Sugar production is an essentialagricultural world product and about 180 milliontons of sugar are produced globally each year with
221ScienceAsia 47 (2021)Thailand capable of supplying abundant sugar up to10 million tons . Many by-products includingsugarcane leaves and sugarcane bagasse (2.4–2.5ton), molasse (0.4–0.5 ton), and filter cake (0.5–0.6ton) are created during 1 ton of sugar and sugaralcohol production, many of which can be recycledfor biofuel and electricity production . Somestudies suggested that the filter cake was suitableas a soil amendment since it has high nutrientcontents . However, its stench and some diseases associated with this material are unfavorableproperties for use. Wastewaters from sugar andethanol production typically contain a high phosphate content that must be reclaimed to mitigatethe environmental problem such as eutrophicationand to allow its reuse as fertilizers . Therefore,filter cake-engineered biochar production could bean effective technology to reuse this agricultural byproduct as an adsorbent for the removal of phosphate from wastewater and to provide available Pin soils.This research aims to investigate the P retentioncapacity of Al- and Fe-biochar prepared from filtercake and to examine P released from Al- and Febiochar applied in acid-washed sand. The obtaineddata will provide useful information on potentialuses of Al- and Fe-biochar in soils with low P contents.Phosphorus sorptionThe P sorption capacity of biochar and filter cakeengineered biochar was investigated to determinethe effects of each metal (Al and Fe) on P sorptioncapacity and its potential reuse as P fertilizer. About0.05 g of each metal-engineered biochar (FBAl andFBFe ) were mixed with 25 ml of separate P solutions (50–1000 mg P/l) in centrifuge tubes. TheP sorption experiment was performed in triplicates.All tubes were shaken in an orbital shaker at roomtemperature (25 2 C) for 48 h. The remaining Pconcentration in the equilibrium solution was determined using the molybdenum blue method aftercentrifugation at 2205g for 15 min. The Langmuirmaximum P sorption coefficient (Q m ) for each engineered biochar was obtained by fitting the sorptiondata using the Langmuir equation as follows:qe Q m K L Ce1 K L Cewhere qe (mg/g) is the amount of P adsorbed tothe solid, Ce (mg/l) is the equilibrium solutionconcentration of dissolved P, and K L is the Langmuirbinding energy constant. The P sorption data werealso modelled using the Freundlich equation as follows:qe K f (Ce )nMATERIALS AND METHODSwhere the coefficient K f and n denote Freundlichaffinity and linearity constants energy, respectively.Preparation of metal-engineered biocharPreparation of phosphorus-laden biocharFilter cake material was obtained from the EasternSugar and Cane Company located in eastern Thailand. For the preparation of filter cake-engineeredbiochar, about 10 g of air-dried filter cake wereseparately impregnated with 60 ml of AlCl3 andFeCl3 solutions (67% w/v) for up to 72 h, dependingon the material saturation time for each metal. Thesaturated material was oven-dried at 80 C for 24 h.The materials were tightly packed into an aluminaceramic crucible. The closed vessel was transferredinto a preheated muffle furnace (600 C) and carbonized under the ambient atmosphere for 1 h. The container was carefully translocated andunheated in a desiccator. Each metal-engineeredbiochar was washed several times with deionized(DI) water to remove impurities and dried at 80 Cfor 24 h. The samples were crushed using an agatemortar, passed through 0.5–2.0 mm sieves, and preserved in airtight containers for further experiments.The Al- and Fe-engineered biochar samples weredesignated as FBAl and FBFe , respectively.After obtaining P sorption data, the metalengineered biochar with high P content designatedas P-laden biochar was produced for incubationexperiments.Briefly, each metal-engineeredbiochar was weighed in separate centrifuged tubesand mixed with the P concentration at 10% ofeach Q m value using a solid:solution ratio of 1:20.The expected concentrations contain reliable Pconcentrations for the P-laden biochar after Pretrieval from the wastewater . The vesselswere agitated on a mechanical shaker at roomtemperature for 48 h. The aliquots were obtainedusing centrifugation at 2205g for 15 min and thendried in the oven at 80 C. All engineered biocharafter P addition was termed as FBAl P and FBFe P .The value of phosphorus-laden biochar pH wasmeasured in water at a solid to solution ratio of 1:2using a pH meter. The total P concentration wasobtained using Aqua regia digestion , followedby P analysis of the extraction using the colorimetricmethod . The produced FBAl P and FBFe P hadwww.scienceasia.org
222ScienceAsia 47 (2021)Table 1 Values of pH and total P concentration (mg/g)in acid-washed sand and P-laden biochar prepared fromfilter cake loaded with Al (FBAl P ) and Fe (FBFe P ).ParameterAcid-washed sandFBAl PFBFe P4.7ND*4.96.05.83.4pHTotal P*ND, not detected.total P content of approximately 6.0 and 3.4 mg/g,respectively (Table 1).Preparation and characterization ofacid-washed sandAcid-washed sand was used as a representative ofsandy soil without nutrients and impurities. Briefly,a bulk sample of the river sand was washed with tapwater to eliminate light fractions of organic matterand suspended clays. The washed sand material wasimmersed in 10% HCl for 24 h to extract remnantelements attached to the particles. The material waswashed at least 3 times with tap water to removethe excess H and Cl– ions caused by the acidwashed procedure. A few drops of silver nitratesolution were used to check for the presence of Cl–ions. The material was washed with DI water afterthe complete removal of Cl– ions and then ovendried for the incubation experiment. Sand pH wasmeasured in water at a solid to solution ratio of 1:1using a pH meter . The total P concentrationwas also analyzed using the above method. Thefield capacity was obtained by using ceramic plateextraction at 0.33 bar . The pH of acid-washedsand was 4.7 with no total P content detected. Thefield capacity of the acid-washed sand sample was3.0% (w/w).Incubation experimentThe incubation technique was used to examine theavailability of P released from the P-laden biocharfor possible use as a P recycling fertilizer in sandysoils that commonly have low P availability. For theincubation experiment, about 5 g of acid-washedsand were weighed in separate centrifuge tubes.The acid-washed sand was incubated with FBAl Pand FBFe P . The investigation identified that theFBAl P and FBFe P in the sand material were due tothe fact that most sandy soils commonly have lowP availability and low water and nutrient retentioncapability. The use of materials with strong P sorption capacities like FBAl P and FBFe P was expectedto release P slowly and thus reduce the P loss byleaching. Each type of engineered biochar waswww.scienceasia.orgplaced in nylon bags with a 100 µm mesh diameter.An application rate of 1% (w/w) was used in thisstudy.The moisture contents of the sand sample weremaintained at 90% of its field capacity for 45 days.The tubes were placed in a controlled osmotic pressure container, which was filled with NaCl solutioncalculated by Jacobus van’t Hoff equation [28, 29].After the desired periods of 7, 30, and 45 days,the samples were taken for determination of thewater-extractable P  and Olsen-extractable Pcontents . Water extraction provides information on the most readily available P pools forplants, whereas the Olsen extraction describes theplant available P pool through the ligand exchangemechanism. The available P fraction calculatedfrom the summation of the water-extractable andOlsen-extractable P was calculated and reported as arelative content of the total P concentration in eachsample. The difference in the available P fractionwith the total P content denotes the long-term Pfraction that is potentially available to plants.RESULTS AND DISCUSSIONPhosphorus sorptionThe maximum P adsorption capacities of all engineered biochar were higher than those of the filtercake biochar (FB). The P sorption data was welldescribed by both the Langmuir and Freundlichmodels with the R2 values in the ranges of 0.76–0.99 (mean 0.91) and 0.94–0.97 (mean 0.96),respectively (Table 2). The FBAl sample had a higherLangmuir maximum sorption capacity (63.7 mg/g)than the FBFe sample (33.2 mg/g, Fig. 1). Comparing these data with existing metal-engineeredbiochar prepared from different feedstocks, the FBFesample had higher P sorption capacity than Febiochar prepared from orange peel pyrolysis at 250to 700 C (Q m 0.22–1.24 mg/g) . The FBAlsample had a lower P retention capacity than theAl-biochar prepared from Cottonwood pyrolyzed600 C (Q m 135 mg/g) . The considerablevariation in the P retention capacity was mainly dueto differences in the metal impurities in each feedstock, which can affect the formations of differenttypes and quantities of metal (oxyhydr)oxides in thebiochar structure that will act as the primary adsorbent for P in the aqueous solution. The LangmuirK L coefficient relating to P binding energy variedconsiderably from 0.003 to 0.33 l/mg. The lowerK L value was found in the FBAl sample, whereasthe higher value was observed in the FBFe samples.
223ScienceAsia 47 (2021)Table 2 Coefficients and correlation coefficients of Langmuir and Freundlich models for P adsorption onto filter cakeengineered biochar loaded with Al (FBAl ) and Fe (FBFe .20.0030.330.990.76FBAlFBFe(mgKf(1–n) nnR223.10.340.170.650.940.97l /g)Q m Langmuir sorption maximum capacity; K L Langmuir binding constant; K f Freundlich affinity constants;and n Freundlich linearity bed P content (mg/g)402000100200300400500(b)30FBFe2010should be carried out to prove this explanation. TheK L coefficients in this study were lower than thoseof Al- and Fe-biochar in previous studies reported as0.012 and 0.046–10.5 l/mg, respectively [11–13].These data reflect that the current metal-biocharsamples could be more easily released P and providehigher available P contents than other reportedmetal-engineered biochar samples.The Freundlich K f coefficient associated withthe quantity of P sorption sites ranged from0.34 mg/g for the FBFe sample to 23.1 mg/g forthe FBAl sample which was lower than that of Albiochar and Fe-biochar of other studies (2971, 10.1,and 1069) [11–13]. The Freundlich n constantindicating the variation of adsorption sites of sorbents differed from 0.17 for the FBAl sample to 0.65for the FBFe sample, while other studies found theFreundlich n constant of Al-biochar at 0.40 andFe-biochar around 0.29–0.87 [11–13]. The lowvalue indicated the adsorption site heterogeneity,and the high value indicated the adsorption sitehomogeneity .Effect of phosphorus-laden biochar onphosphorus availability00100200300400500P in solution (mg/l)Fig. 1 Phosphorus adsorption isotherms of filter cakeengineered biochar: (a) FBAl and (b) FBFe . Symbols showexperimental data, and error bars are standard errors oftriplicate measurements.These results suggested the low and high P bindingenergy for the FBAl and FBFe samples, respectively.The difference between K L constant for FBAl andFBFe samples might be attributable to the variation in crystal sizes of metal oxides formed in theengineered biochar that controlled magnitudes ofspecific surface area and chemical surface reactivityof the adsorbents. However, further investigationThe results of testing for water-extractable andOlsen-extractable P in the acid-washed sand after 45 days of incubation with Al- and Fe-biocharare provided in Fig. 2. Different metal-engineeredbiochar samples released varied water-extractableand Olsen-extractable P contents into the sand sample. The acid-washed sand containing Al-biocharhad water-extractable P of 0.1–0.5 mg/kg whereasthe acid-washed sand contained Fe-biochar withwater-extractable of 0.7–1.6 mg/kg (Fig. 3).The Olsen-extractable P for the acid-washedsand in the Al-biochar series was somewhat stable over the 45 days of the incubation (11.4 to12.4 mg/kg) while that in the Fe-biochar series wasconsiderably increased during the incubation period(9.1 to 19.2 mg/kg). The constant release of available P from Al-biochar may be due to the more stablewww.scienceasia.org
224ScienceAsia 47 (2021)Table 3 Water-extractable and Olsen-extractable P contents in acid-washed sand over 45 days of incubation with Al(FBAl P ) and Fe-biochar (FBFe P ).Available P (mg/kg)ExtractionFBAl P treatmentWaterOlsenFBFe P treatmentDay 7Day 30Day 45Day 7Day 30Day 450.5 0.0111.4 2.740.1 0.0811.7 0.950.2 0.0712.4 1.631.1 0.039.1 1.570.7 0.0214.0 2.611.6 0.4119.2 1.70Water extractionOlsen extraction(a)25Sand FBAl-P (1%)2015P concentration (mg/g)10507253045(b)Sand FBFe-P (1%)2015105073045DaysFig. 2 Water- and Olsen-extractable P concentration ofacid-washed sand treated with (a) FBAl P and (b) FBFe P .Bar graphs show experimental data, and error bars arestandard errors of triplicates.phase of Al oxides in the engineered biochar sample,whereas the increasing P concentration releasedwith time from Fe-biochar is consistent with theheterogeneity of the adsorption sites of the biocharthat may control different P release behaviors fromthe Fe-biochar sample. Interestingly, the high Olsenwww.scienceasia.orgextractable P values in the Al- and Fe-biochar series suggest the possible uses of the Al- and Febiochar samples, which are typically thought to beunsuitable for plant use, for improving the availableP content in sandy soils with a low native P. Therelease of P from the Al- and Fe-biochars could havebeen due to the replacement of orthophosphate ions–(H2 PO–4 or HPO2–4 ) with HCO3 ions by the ligandexchange process. This exchange process resemblesthe release of HCO–3 ions from plant roots to acquireanions . The data were consistent with recentresearch demonstrating that the uses of Fe(II)- andFe(III)-biochar could improve P availability in paddythrough the reductive dissolution of Fe oxides inbiochar upon flooding .In general, Olsen-extractable P is consideredto be available for plant uptake . Considering extractable P from all metal-engineered biocharsamples (FBAl P and FBFe P ) treated in the acidwashed sand with the low total and available Pcontent, the results demonstrated that the concentration of the Olsen-extractable P in all incubationseries was typically greater than the critical valuefor corn production as assessed using Olsen extraction of 5.0 mg/kg . The data suggestedthat applications of FBAl P and FBFe P at the rateof 1% (w/w), corresponding to 19.50 ton/ha insoils, could provide sufficient amounts of availableP for the entire period of productions for certaineconomic crops such as corn.Moreover, the available P pools (calculated fromboth water- and Olsen-extractable P) were very lowcompared to the total P in each metal-P biochar. Therelative fraction of available P was just 0.20–0.21%and 0.30–0.61% of the total P for the FBAl P andFBFe P biochar samples, respectively, which werecontinuously released to the sand during the 45day incubation (Fig. 3). Other studies of P releasefrom metal-engineered biochar by similar production were focused mainly on single extraction fromMg-biochar, in which 0.01 to 14% of their total Pcan be extracted by citric acid, KCl, and Mehlich-3[37–39]. These data reflect that substantial fractions of reserved P pools could have remained in the
225ScienceAsia 47 (2021)Available P (% of total P)0.80Sand FBAl-PSand FBFe-P0.60required further investigation in various soil andplant types in pot experiments or field scales beforerecommending its application.CONCLUSION0.400.200.00730Days45Fig. 3 Relative percentage (% of total P) of available Pcontent (water and Olsen extractable) for P-laden biocharprepared from filter cake loaded with Al (FBAl P ) and Fe(FBFe P ). Bar graphs show experimental data.biochar samples and could be potentially availablein the long term if the soil conditions are suitable forthe dissolution or exchange of P from host phases(Al-P and Fe-P compounds) in the biochar samples.Economic and environmental aspectsPhosphate mineral resource limitation, soil P fixation, and P contamination from excessive fertilization have called great attention to effective phosphate fertilizer use for agricultural and environmental sustainability. Recycle, reuse, and recovery arenecessary for agriculture and industries, includingthe sugar industry . A utilization of filter cake,an effective by-product in the sugar industry, asan adsorbent for phosphate contaminant recoveryand subsequently recycle into agricultural lands asP fertilizer could be an effective technology to solvethis issue. Costs related to metal-engineered biocharproduction are derived from modification processes(metal impregnation and pyrolysis), while severalbenefits are waste recycling, water contaminantreduction, and decreasing P fertilizer cost. However,in real practice, biochar engineering could be developed to be cheaper and more effective technology.Applications of biochar-based pollutant removersrequired more investigation to unravel such adverse impacts of toxic pollutants from a water body.Furthermore, possible real operating systems (i.e.,natural water body or industrial water treatmentsystem) remain to be improved for future uses. Theapplication of P-laden biochar-based P fertilizer alsoThe Al- and Fe-engineered biochar samples prepared from filter cake, a main by-product of thesugar industry, showed excellent P sorption capacityfrom aqueous solution. The P retention competencyof the Fe-biochar was better than that of biocharprepared from orange peel biomass from reportedstudies. The Al-biochar from the current study hada lower P retention potential than cottonwood-Albiochar. However, the metal-biochar incorporationinto sand material showed that a sufficient fractionof Olsen-extractable P could be regularly released.The extracted P content from the metal biocharwas only approximately 1% of their total P content,indicating that a substantial amount of the P fractionremained in the biochar matrix and could be considered a long-term source and sink of P for plantuse. This study has shed light on the possible useof Al- and Fe-biochar for improving P availabilityin sandy soils that are typically low in water andnutrient retention capacity. The P reclamation fromwastewater using both Al-and Fe- biochars and theirsubsequent incorporation as P fertilizers in sandysoils under the field condition should be furtherinvestigated.Acknowledgements: The authors thank the KasetsartUniversity Research and Development Institute (KURDI),Bangkok, Thailand for research funding (Grant No.18.58).REFERENCES1. Lehmann J, Joseph S (2015) Biochar for Environmental Management, Saxon Graphics Ltd, NY, USA.2. Sohi S, Lopez-Capel E, Krull E, Bol R (2009) Biochar,climate change and soil: a review to guide future research. CSIRO Land and Water Science Report 05/09,CSIRO, Australia.3. Mohan D, Abhishek K, Sarswat A, Patel M, Singh P,Pittman CU (2018) Biochar production and applications in soil fertility and carbon sequestration: asustainable solution to crop-residue burning in India.RSC Adv 8, 508–520.4. Ahmad M, Rajapaksha AU, Lim JE, Zhang M, BolanN, Mohan D, Vithanage M, Lee SS, et al (2014)Biochar as a sorbent for contaminant managementin soil and water: a review. Chemosphere 99, 19–33.5. Lee C, Lim W (2006) Variation of harmful algal blooms in Masan-Chinhae Bay. ScienceAsia 32,51–56.www.scienceasia.org
2266. Zheng YL, Gao B (2019) Reclaiming phosphorusfrom secondary treated municipal wastewater withengineered biochar. Chem Eng J 362, 460–468.7. Yao Y, Gao B, Chen JJ, Yang LY (2013) Engineered biochar reclaiming phosphate from aqueoussolutions: mechanisms and potential applicationas a slow-release fertilizer. Environ Sci Technol 47,8700–8708.8. Vikrant K, Kim K-H, Ok YS, Tsang DC, Tsang YF, GiriBS, Singh RS (2018) Engineered/designer biocharfor the removal of phosphate in water and wastewater. Sci Total Environ 616, 1242–1260.9. Chaiyaraksa C, Lokham N, Kuikrong R, Artsanapaiboon S (2020) Immobilization of cadmium in soilusing magnetic biochar derived from Eichhornia crassipes. ScienceAsia 46, 450–456.10. Chen QC, Qin JL, Sun P, Cheng ZW, Shen GQ (2018)Cow dung-derived engineered biochar for reclaimingphosphate from aqueous solution and its validationas slow-release fertilizer in soil crop system. J CleanerProd 172, 2009–2018.11. Zhang M, Gao B (2013) Removal of arsenic,methylene blue, and phosphate by biochar/AlOOHnanocomposite. Chem Eng J 226, 286–292.12. Ajmal Z, Muhmood A, Usman M, Kizito S, Lu J, DongR, Wu S (2018) Phosphate removal from aqueoussolution using iron oxides: Adsorption, desorptionand regeneration characteristics. J Colloid InterfaceSci 528, 145–155.13. Chen BL, Chen ZM, Lv SF (2011) A novel magneticbiochar efficiently sorbs organic pollutants and phosphate. Bioresour Technol 102, 716–723.14. Abdala DB, da Silva IR, Vergutz L, Sparks DL (2015)Long-term manure application effects on phosphorusspeciation, kinetics and distribution in highly weathered agricultural soils. Chemosphere 119, 504–514.15. Suriyagoda L, De Costa W, Lambers H (2014) Growthand phosphorus nutrition of rice when inorganicfertiliser application is partly replaced by straw undervarying moisture availability in sandy and clay soils.Plant Soil 384, 53–68.16. Borchard N, Wolf A, Laabs V, Aeckersberg R, SchererH, Moeller A, Amelung W (2012) Physical activationof biochar and its meaning for soil fertility and nutrient leaching: a greenhouse experiment. Soil UseManage 28, 177–184.17. Bruun EW, Petersen CT, Hansen E, Holm JK,Hauggaard-Nielsen H (2014) Biochar amendmentto coarse sandy subsoil improves root growth andincreases water retention. Soil Use Manage 30,109–118.18. Lehmann J, Rondon M (2006) Biological Approachesto Sustainable Soil Systems, CRC Press/Taylor & Francis Group, Florida, USA.19. USDA (2020) Sugar: World Markets and Trade.Foreign Agricultural Service.20. Chauhan MK, Chaudhary S, Kumar S (2011) Lifewww.scienceasia.orgScienceAsia 47 .36.cycle assessment of sugar industry: A review. RenewSust Energ Rev 15, 3445–3453.Prado RdM, Caione G, Campos CNS (2013) Filtercake and vinasse as fertilizers contributing to conservation agriculture. Appl Environ Soil Sci 2013, ID581984.Poddar PK, Sahu O (2017) Quality and managementof wastewater in sugar industry. Appl Water Sci 7,461–468.Klüpfel L, Piepenbrock A, Kappler A, Sander M(2014) Humic substances as fully regenerable electron acceptors in recurrently anoxic environments.Nat Geosci 7, 195–200.Chen M, Ma LQ (2001) Comparison of three aquaregia digestion methods for twenty Florida soils. SoilSci Soc Am J 65, 491–499.Murphy J, Riley JP (1962) A modified single solutionmethod for the determination of phosphate in natural waters. Anal Chim Acta 27, 31–36.Sparks DL, Page A, Helmke P, Loeppert R, Soltanpour P, Tabatabai M, Johnston C, Sumner M (1996)Methods of Soil Analysis, Part 3 – Chemical Methods,American Society of Agronomy, Inc., Soil ScienceSociety of America, Inc., USA.Klute A (1986) Water retention: laboratory methods.In: Klute A (ed) Methods of Soil Analysis: Part 1 Physical and Mineralogical Methods, 2nd Edn, AmericanSociety of Agronomy, Inc., Soil Science Society ofAmerica, Inc., USA, pp 635–662.Van’t Hoff JH (1887) Die Rolle des osmotischenDruckes in der Analogie Zwischen Losungen undGasen. Z Physik Chemie 1, 481–493.Feher JJ, Ford GD (1995) A simple student laboratoryon osmotic flow, osmotic pressure, and the reflectioncoefficient. Adv Physiol Educ 268, 10–20.Yusiharni E, Gilkes RJ (2012) Minerals in the ash ofAustralian native plants. Geoderma 189, 369–380.Olsen SR (1954) Estimation of Available Phosphorusin Soils by Extraction with Sodium Bicarbonate, USDepartment of Agriculture, USA.Sposito G (1980) Derivation of the Freundlich equation for ion exchange reactions in soils. Soil Sci SocAm J 44, 652–654.Kollist H, Jossier M, Laanemets K, Thomine S(2011) Anion channels in plant cells. FEBS J 278,4277–4292.Wu, LP, Zhang, SR, Wang, J, Ding XD (2020) Phosphorus retention using iron (II/III) modified biocharin saline-alkaline soils: Adsorption, column and fieldtests. Environ Pollut 261, ID 114223.Menon R, Chien S, Hammond L (1990) Development and evaluation of the Pi soil test for plantavailable phosphorus. Commun Soil Sci Plant Anal21, 1131–1150.Mallarino A, Blackmer A (1992) Comparison ofmethods for determining critical concentrations ofsoil test phosphorus for corn. Agron J 84, 850–856.
ScienceAsia 47 (2021)37. Fang C, Zhang T, Li P, Jiang RF, Wang YC (2014)Application of magnesium modified corn biochar forphosphorus removal and recovery from swine wastewater. Int J Environ Res Public Health 11, 9217–9237.38. Takaya CA, Fletcher LA, Singh S, Okwuosa UC,Ross AB (2016) Recovery of phosphate with chemically modified biochars. J Environ Chem Eng 4,1156–1165.39. Yao Y, Gao B, Chen J, Yang L (2013) Engineered227biochar reclaiming phosphate from aqueous solutions: mechanisms and potential application asa slow-release fertilizer. Environ Sci Technol 47,8700–8708.40. Soltangheisi A, Withers PJA, Pavinato PS, CherubinMR, Rossetto R, Do Carmo JB, da Rocha GC, Martinelli LA (2019) Improving phosphorus sustainability of sugarcane production in Brazil. Glob ChangeBiol Bioenergy 11, 1444–1455.www.scienceasia.org
Aluminum- and iron-engineered biochar from sugarcane ﬁlter cake as phosphorus adsorbents and fertilizers . Biochar is a carbon-rich material with high stability produced by the carbonization of biomass under limited oxygen [1,2]. . for possible use as a P recycling fertilizer in sandy